orientationdensityfunction …rahi/paper/jac2007.pdfto be more precise, let ðgÞ¼ ~½!ðgg1 0...
Embed Size (px)
TRANSCRIPT

electronic reprint
Journal of
AppliedCrystallography
ISSN 00218898
Editor: Gernot Kostorz
Orientation density functioncontrolled pole probability density function measurements: automated adaptive control of texture goniometers
Helmut Schaeben, Ralf Hielscher, JeanJacques Fundenberger, Daniel Potts andJürgen Prestin
Copyright © International Union of Crystallography
Author(s) of this paper may load this reprint on their own web site provided that this cover page is retained. Republication of this article or itsstorage in electronic databases or the like is not permitted without prior permission in writing from the IUCr.
J. Appl. Cryst. (2007). 40, 570–579 Helmut Schaeben et al. � ODFcontrolled PDF measurements

research papers
570 doi:10.1107/S0021889807019711 J. Appl. Cryst. (2007). 40, 570–579
Journal of
AppliedCrystallography
ISSN 00218898
Received 12 February 2007
Accepted 20 April 2007
# 2007 International Union of Crystallography
Printed in Singapore – all rights reserved
Orientation density functioncontrolled poleprobability density function measurements:automated adaptive control of texture goniometers
Helmut Schaeben,a* Ralf Hielscher,a JeanJacques Fundenberger,b Daniel Pottsc
and Jürgen Prestind
aGeoscience Mathematics and Informatics, Freiberg University of Mining and Technology,
Germany, bLaboratoire d’Etude des Textures et Application aux Materiaux, UMR CNRS 7078,
Université de Metz, France, cMathematics, Chemnitz University of Technology, Germany, anddMathematics, Lübeck University, Germany. Correspondence email: [email protected]
A novel control of a texture goniometer, which depends on the texture being
measured itself, is suggested. In particular, it is suggested that the obsolete
control with constant step sizes in both angles is replaced by an adaptive
successive refinement of an initial coarse uniform grid to a locally refined grid,
where the progressive refinement corresponds to the pattern of preferred
crystallographic orientation. The prerequisites of this automated adaptive
control is the fast inversion of pole intensities to orientation probabilities in the
course of the measurements, and a mathematical method of inversion that does
not require a raster of constant step sizes and applies to sharp textures.
1. Motivation and introduction
1.1. Crystallographic orientation
Texture analysis is the analysis of preferred crystallographic
orientation in polycrystalline materials. Neglecting crystal
symmetry or assuming triclinic crystal symmetry, the crystal
lographic orientation g of an individual crystal is the active
orthogonal transformation g 2 Oð3Þ which brings an orthogonal coordinate system KS ¼ hx; y; zi fixed to the specimeninto coincidence with an orthogonal coordinate system
KC ¼ ha; b; ci fixed to the crystal,g 2 Oð3Þ : KS 7!KC;
in the sense that
g x ¼ a; g y ¼ b; g z ¼ c:Then the vector rKS of coordinates with respect to KS of aunique vector v and the vector hKC of its coordinates with
respect to KC are related to one another by
g hKC ¼ rKS :It should be noted that handedness is not generally preserved.
In the case of crystal symmetry, several symmetrically
equivalent crystal coordinate systems KC;K0C exist, which can
be distinguished mathematically but not physically. If Gpointdenotes the point group of the crystal symmetry class, then the
set of crystallographically equivalent orientations is repre
sented by the coset gGpoint. As a result of Friedel’s law the
effective crystal symmetry imposed by any diffraction
experiment is described by the point group
GLaue ¼ Gpoint � fid;�idg;
which is also referred to as the Laue class (here id denotes the
identity, and �id the inversion). SinceOð3Þ=GLaue ¼ SOð3Þ=½GLaue \ SOð3Þ�;
the cosets of equivalent orientations with respect to the
effective symmetry imposed by the diffraction experiment can
be represented by proper rotations in SO(3) only. Therefore
all considerations are restricted to SO(3).
1.2. Orientation and pole probability density function
The major subject of texture analysis is the orientation
probability density function (ODF) f , as it allows the deter
mination of anisotropic macroscopic material properties from
the corresponding singlecrystal properties. More specifically,
texture analysis is the analysis of patterns of preferred crys
tallographic orientation of a polycrystalline specimen given
in terms of its orientation probability density function
f : SOð3Þ ! gþ defined as
f ðgÞ ¼ Vg=Vdg
; ð1Þ
where V denotes the total volume of the specimen, Vg the
volume of crystallites carrying the orientation g, and dg the
Haar measure on SOð3Þ. In order to model crystal symmetrygiven by a Laue group GLaue � Oð3Þ, the ODF f is defined tosatisfy the symmetry relations
f ðgÞ ¼ f ðg g0Þ; g0 2 GLaue \Oð3Þ:With Xray (including synchrotron) or neutron diffraction
experiments, the orientation density f cannot be measured
directly; only integral information concerning f can be
sampled. More precisely, ‘pole figures’
electronic reprint

Pðh; rÞ ¼ 14�
ZGðh;rÞ [Gð�h;rÞ
f ðgÞ dg; ðh; rÞ 2 S2 � S2 ð2Þ
are experimentally accessible with a texture goniometer for
discrete directions hi; rji 2 S2, where S2 denotes the unitsphere in R3]. The path of integration Gðh; rÞ is defined as thefibre
Gðh; rÞ ¼ g 2 SOð3Þ j g h ¼ r; ðh; rÞ 2 S2 � S2� �:Interpreting r rather as a parameter than as a variable, the
function h 7!Pðh; rÞ is the probability density functionproviding the probability that the crystallographic direction
(‘pole’) h statistically coincides with the macroscopic specimen
direction r.
The basic term of the mathematical model of texture
goniometry is the onedimensional totally geodesic Radon
transform
Rf ðh; rÞ ¼ 12�
ZGðh;rÞ
f ðgÞ dg; ðh; rÞ 2 S2 � S2; ð3Þ
which associates to an orientation probability density function
f on SOð3Þ its mean values along the onedimensionalgeodesics Gðh; rÞ and
Pðh; rÞ ¼ 12
hRf ðh; rÞ þ Rf ðh;�rÞ
i¼ X f ðh; rÞ; ð4Þ
which is called the basic crystallographic Xray transform even
though it does not depend on the radiation used for diffrac
tion. Notationally, we do not distinguish between experimen
tally accessible pole figures and the basic crystallographic
Xray transform, which differ just by a summation over crys
tallographically symmetrically equivalent directions.
1.3. Poletoorientation density inversion
In practice, the problem is to recover a reasonable
approximation of the orientation probability density function
f from experimental intensities
�ij ¼ �ðhi; rji Þ ¼ aðhiÞPðhi; rjiÞ þ bðhiÞ;ji ¼ 1; . . . ; Ji; i ¼ 1; . . . ; I; ð5Þ
modelled by pole probability density functions (PDFs) P with
constants aðhiÞ; bðhiÞ 2 R depending on the crystal form. Theindices indicate that there is no regular grid of positions ðhi; rjiÞimposed, but that the specimen positions rji may depend on
the crystal form hi and may be different for each crystal form.
From integral geometry it is well known that the totally
geodesic Radon transform possesses a unique inverse under
mathematically mild assumptions (cf. Helgason, 1984, 1999).
As a result of the additional symmetry introduced by the
diffraction experiment itself, the basic crystallographic Xray
transform is not generally invertible, and therefore neither are
the pole probability density functions (Matthies, 1979). To
resolve the inverse problem of texture analysis, additional
modelling assumptions are required. Here we apply a first
modelling assumption that the true orientation probability
density function f : SOð3Þ ! Rþ be expanded into a finiteseries of given radially symmetric basis functions, the Radon
transform of which is analytically known.
research papers
J. Appl. Cryst. (2007). 40, 570–579 Helmut Schaeben et al. � ODFcontrolled PDF measurements 571
Figure 2The von Mizes–Fisher kernel for � ¼ 7:5 (a), its Radon transform (b) onthe spatial domain and their spectral representation on the frequencydomain (c).
Figure 1The de la Vallée Poussin kernel for � ¼ 13 (a), its Radon transform (b) onthe spatial domain and their spectral representation on the frequencydomain (c).
electronic reprint

To be more precise, let
ðgÞ ¼ ~ ½!ðg g�10 Þ�; !ðgg�10 Þ ¼ arccostrace gg�10 �1
2; ð6Þ
be a nonnegative, radially symmetric function on SOð3Þ, welllocalized around its centre g0 2 SOð3Þ that is monotonouslydecreasing with respect to the angular distance !ðg; g0Þ of gfrom g0. Then the halfwidth b 2 ð0; 1Þ of is defined by
~ ðbÞ ¼ 12~ ð0Þ:
Furthermore, let g1; . . . ; gM 2 SOð3Þ be an approximateequidistribution in SOð3Þ with resolution � =minm 6¼m0 !ðgmg�1m0 Þ. Then we apply the first model assumptionthat there are coefficients c 2 RMþ such that
f ðgÞ ’XMm¼1
cm ½!ðg g�1m Þ�: ð7Þ
Examples of suitable radially symmetric functions are the de la
Vallée Poussin kernel
~ �ð!Þ ¼Bð 32 ; 12 Þ
Bð 32 ; �þ 12 Þcos2�ð!=2Þ; ! 2 ð0; �Þ; � 2 R; ð8Þ
where B denotes the � function, and the von Mizes–Fisherkernel
~ �ð!Þ ¼1
I 0ð�Þ � I 1ð�Þexpð� cos!Þ; ! 2 ½0; ��;
where I n, n 2 N0 denote the modified Bessel functions of thefirst kind,
I nð�Þ ¼1
�
Z�
0
expð� cos!Þ cos n! d!; � 2 Rþ:
The de la Vallée Poussin kernel is of special interest as its
Fourier coefficients not only decrease smoothly, but also
eventually vanish, i.e. its harmonic
series expansion is finite. Moreover, its
form is preserved under the Radon
transform, i.e. the Radon transform of
the de la Vallée Poussin kernel on
SOð3Þ is the de la Vallée Poussinkernel for S2 � S2 (Schaeben, 1997,1999; Hielscher, 2007). It is well
known that radial symmetry is
preserved by the Radon transform.
Then, from a practical point of view it
seems sensible to choose radially
symmetric basis functions that are
easily numerically tractable. For both
kernel functions mentioned above
there are simple explicit formulae for
their Radon transforms, i.e. we have
R �ðh; rÞ ¼ ð1þ �Þ cos2� ffðg0h; rÞ=2in the case of the de la Vallée Poussin
kernel and
R �ðh; rÞ ¼I 0
��2 ½1þ cos ffðgh; rÞ�
�I 0ð�Þ � I 1ð�Þ
� exp��
2½�1þ cos ffðgh; rÞ�
�
in the case of the von Mizes–Fisher
kernel.
Plots of the de la Vallée Poussin
kernel and the von Mizes–Fischer
kernel are given in Figs. 1 and 2.
Since the Radon transform is linear,
its application to the superposition of
radially symmetric functions described
in equation (7) results in
Rf ðh; rÞ ¼ PMm¼1
cmR �ðgmh; rÞ:
research papers
572 Helmut Schaeben et al. � ODFcontrolled PDF measurements J. Appl. Cryst. (2007). 40, 570–579
Figure 3Successive refinement of measurement positions in k steps, where k enumerates the rows.
electronic reprint

The numerical resolution of the inverse Radon transform is
accomplished by fitting the coefficients cm;m ¼ 1; . . . ;M, tothe measured intensities subject to the additional modelling
assumptions that cm � 0; k ¼ 1; . . . ;M, to guarantee nonnegativity.
Since the inverse of the basic crystallographic Xray trans
form is not well defined, we introduce as yet another model
ling assumption the maximum smoothness of the orientation
probability density function to be recovered. Here we suggest
the measurement of smoothness in terms of derivatives of f , or
more generally in terms of norms of f with respect to appro
priately constructed Sobolev spacesH½SOð3Þ� (Hielscher et al.,2005). The nonlinear problem to be solved then reads
~cc ¼ argminXIi¼1
XJiji¼1
XMm¼1
aðhiÞ cmR �ðgmhi; rji Þ þ bðhiÞ � �ij�����
�����2
þ �XMm¼1
cm �ð g�1m ÞH½SOð3Þ������
�����2
; ð9Þ
where � is the parameter of regularization weighting thepenalty term.
To solve equation (9), methods of fast matrixvector
multiplication are combined with iterative methods. Fast
Fourier transforms are an option for the fast matrixvector
multiplication; alternatively, multipole or multigrid methods
may be used. The modified steepest
descent algorithm provides an iterative
solution for the nonnegative
constrained optimization problem, and
so do the Richardson–Luci, gradient
projection residual norm (GPRN) and
gradient projection residual norm
conjugated gradients (GPRNCG)
methods (cf. Bardsley & Vogel, 2003).
The method may be seen as a
generalization of the classical harmonic
method initialized by Bunge (1965) and
Roe (1965) and discussed by Schaeben
(2000), or the texture component fit
method (Grewen & Wassermann, 1955;
Virnich et al., 1978; Lücke et al., 1981,
1986; Bukharova & Savyolova, 1985a,b;
Nikolayev et al., 1992; Helming &
Eschner, 1990; Eschner, 1993, 1994),
depending on the point of view
(Schaeben & Boogaart, 2003). While a
preliminary sketch was presented by
Schaeben (1996) and Hielscher &
Schaeben (2006), the method is fully
developed by Hielscher (2007). It
should be noted that our generalization
may expand an orientation probability
density function into up to 300 000
symmetrized radially symmetric basis
functions, each with a halfwidth of
1.5. It does not require a raster ofconstant step sizes for the measured
intensities and applies to extremely
sharp textures. The method will be
comprehensively presented elsewhere
in a forthcoming paper.
2. Automated adaptivelycontrolled texture goniometry
In what follows, ðhk‘Þ are the Millerindices of a crystallographic lattice
plane with normal vector h, and fhk‘gdenotes the crystal form of lattice
research papers
J. Appl. Cryst. (2007). 40, 570–579 Helmut Schaeben et al. � ODFcontrolled PDF measurements 573
Figure 4Computed PDFs after the kth turn of measurement, where k enumerates the rows.
electronic reprint

planes symmetrically equivalent to ðhk‘Þ.Texture analysis employs the effect of diffraction of radia
tion (Xrays including synchrotron, neutrons, electrons) at the
crystallographic lattice planes. It is based on the Bragg
equation
n� ¼ 2dfhk‘g sin#fhk‘g; n 2 N:For a monochromatic beam of wavelength � and a constant#fhk‘g, the diffracted intensity is a measure of the volumeportion of crystals for which the bisecting line between the
initial and diffracted beam is orthogonal to lattice planes with
lattice spacing dfhk‘g. Then the diffracted intensity recordedwith a conventional detector is a statistical measure of the
frequency by volume that a given crystallographic direction
agrees with a given specimen direction r 2 S2. With adiffractometer with a texture goniometer, the specimen can be
rotated in such a way that each normal h of lattice planes with
spacing dfhk‘g satisfies this condition once. Thus, the diffractionexperiment results for a lattice plane given in terms of its
Miller indices fhk‘g in a statistical distribution of intensitiesPðh; rÞ on the fhk‘gpole sphere, which is referred to as thefhk‘gpole figure in texture analysis.
In the early days of texture analysis, the rotation of the
specimen with the texture goniometer used to be controlled by
step motors such that intensity measurements were performed
with respect to a regular raster of measuring positions with a
constant step size �’ in the azimuth ’ and a constant step size�� in the pole (tilt) angle �, or with respect to a regular rasterof measuring positions with a constant step size along a spiral.
Thus the specimen directions of measurements are geome
trically arranged in a regular grid, with the former control in a
grid of points
rij ¼ ðsin i�’ sin j��;cos i�’ sin j��; cos j��Þt;
i ¼ 0; 1; . . . ; 2��’
� �;
j ¼ 0; 1; . . . ; �2��
� �: ð10Þ
With �’ ¼ �� ¼ 5, an incompletelymeasured pole figure with 0 ’
360, 0 � 70 comprises 1008 positions of measurements. Nowadays the
rotation of the specimen is controlled
by a step motor and a personal
computer. However, the major
features of the experiment have been
conserved: (i) the sequence of posi
tions is fixed before the experiment is
started and thus independent of the
progress of the measurements, and (ii)
the measurements are geometrically
arranged in a regular grid. An
obviously poor property of this kind of
regular grid is the varying spatial
resolution of the pole sphere.
Presumably, regular grids of the type
represented by equation (10) are still
used because commercial software
packages for texture analysis accom
panying diffractometers with a texture
goniometer require data confined to
such grids, even though more appro
priate grids, in particular approxi
mately spherically uniform grids, have
been suggested and successfully
applied in practical tests (Tarkowski et
al., 2004).
Traditionally, the single most
prominent goal of texture analysis is to
recover a reasonable approximation ~ffof the orientation probability density
research papers
574 Helmut Schaeben et al. � ODFcontrolled PDF measurements J. Appl. Cryst. (2007). 40, 570–579
Figure 5Estimated ODF after intial measurements.
electronic reprint

function f from experimental polefigure intensities �, cf.equation (5). Usually an orientation probability density ~ff iscomputed after the experiment is finished.
Alternatively, we suggest a novel control of a texture
goniometer which depends on the texture being measured
itself. In particular, we suggest replacing the obsolete control
with constant step sizes in both angles by an adaptive
successive refinement of an initial coarse uniform grid to a
locally refined grid where the progressive refinement corre
sponds to the pattern of preferred crystallographic orienta
tion. Hence, our novel control differs in two essentials from
the conventional control: (i) the sequence of positions is not
fixed but incomplete when the experiment is started and
depends on the progress of the experiment, and (ii) the
successive refinement of positions depends on the actually
observed pattern of preferred crystallographic orientation and
its simultaneous analysis in terms of successively improved
approximations of the orientation probability density function
with respect to the most recent refinement, and does not result
in a regular grid. Thus measurements and computations
of orientation probability density functions are mutually
dependent. The prerequisite of this automated adaptive
control is the fast inversion of experimental pole intensities to
mathematically modelled orientation probabilities in the
course of the measurements, and a mathematical method of
inversion that does not require a raster of constant step sizes
and which applies to sharp textures. The automated adaptive
control of the texture goniometer is especially well suited for
the capture, mathematical representation and analysis of
sharp textures.
The experiment commences with a list of initial positions
according to a coarse approximately uniform grid. This list is
processed by the personal computer controlling the texture
goniometer and directed to the step motor. During the first
turn of measurements intensities with respect to this initial
grid of positions are recorded. These polefigure intensities are
inverted to the initial approximation of
an orientation probability density
function according to the method
given by equation (9). This first
approximation is analysed to deter
mine regions of the hpole spheres of
special interest where the initial grid
should be refined locally. Criteria for
refinement may be
(i) values of the computed pole
probability density function larger
than a userdefined threshold,
(ii) a difference of measured and
computed pole probability density
functions larger than a userdefined
threshold,
(iii) values of the gradient of the
computed pole probability density
function larger than a userdefined
threshold,
(iv) values of the Laplacian of the
computed pole probability density
function larger than a userdefined
threshold, or
(v) any other sensible property.
The value of the threshold may be
constant or change with the turn of the
measurements. The criteria may be
chosen alternatively or may be
combined in an hierarchical or
weighted manner.
The additional positions of the
locally refined grid are then added to
the list of positions controlling the
texture goniometer and directed to the
step motor. In the second turn of
measurements, intensities with respect
to these additional positions are
recorded. Depending on the construc
research papers
J. Appl. Cryst. (2007). 40, 570–579 Helmut Schaeben et al. � ODFcontrolled PDF measurements 575
Figure 6Estimated ODF after the first refinement.
electronic reprint

tion of the diffractometer and the
goniometer, the sequence of the posi
tions may be optimized to minimize the
total motion of the specimen or the
total time of the second turn. The new
intensities are entered into the inver
sion and start the computation of an
improved approximation of an orien
tation probability density function. The
first computed approximation is now
used as initial solution of the optimi
zation problem given by equation (9).
Its renewed analysis results in an
updated local refinement or in a
progressive local refinement of the
same regions of the pole spheres. These
new positions are again added to the
list of positions, and the experiment is
continued by a third turn of measure
ments with respect to these additional
positions. The turns of measurement
and computations are terminated if
(i) the criteria for refinement are
exhausted,
(ii) the approximation of an orien
tation probability density function
cannot be improved, or
(iii) the technical limitations of the
diffractometer or the texture goni
ometer are reached.
The advantage of this automated
adaptive control is an efficient experi
mental design. More specifically, our
design provides a maximum of infor
mation within a minimum period of
time or an optimum use of the avail
able period of time for measurements.
Finally, extremely sharp textures can
be efficiently captured, represented
and analysed with this approach. In the case of a ‘technical
single crystal ’, an efficient starting grid would be a very coarse
grid already locally refined in a sufficiently large neighbour
hood of the expected peak position (and its crystal symmetry
equivalents), which is usually known a priori.
2.1. Flow chart
(1) Choose crystal directions h1; . . . ; hN 2 S2 for polefiguremeasurements.
(2) Initialize k 0.(3) Set initial resolution �ðkÞ.(4) Define initial coarse grid of specimen directions
rðkÞiji2 S2, i ¼ 1; . . . ;N, ji ¼ 1; . . . ; JðkÞi with resolution �ðkÞ.
(5) Measure diffraction intensities �ðkÞiji , i ¼ 1; . . . ;N,ji ¼ 1; . . . ; JðkÞi .
(6) Estimate ODF f ðkÞ by solving PDFtoODF inversionproblem.
Fix an approximate equidistribution gðkÞ1 ; . . . ; g
ðkÞMk
in
SOð3Þ=GLaue with resolution 32 �ðkÞ.Fix a radially symmetric function � with halfwidth
b ¼ �ðkÞ.Determine coefficients cðkÞm , m ¼ 1; . . . ;MðkÞ of the ansatz
[equation (7)] by solving the minimization problem equation
(9).
(7) Stop if termination criteria are satisfied, e.g. if the
maximum resolution of the texture goniometer is reached or
the estimate f ðkÞ sufficiently explains the texture.(8) Refine resolution �ðkþ1Þ ¼ 12 �ðkÞ.(9) Define grids of specimen directions r
ðkþ1Þiji2 S2,
i ¼ 1; . . . ;N, ji ¼ 1; . . . ; Jðkþ1Þi , with resolution �ðkþ1Þ byrefining the grids r
ðkÞiji2 S2, i ¼ 1; . . . ;N, ji ¼ 1; . . . ; JðkÞi .
(10) Calculate criteria of refinement for all new specimen
directions rðkþ1Þiji 2 S2, i ¼ 1; . . . ;N, ji ¼ 1; . . . ; Jðkþ1Þi (e.g.
lower bound for computed PDF, gradient of the PDF at these
directions etc.) based on the current estimate of the ODF f ðkÞ.
research papers
576 Helmut Schaeben et al. � ODFcontrolled PDF measurements J. Appl. Cryst. (2007). 40, 570–579
Figure 7Estimated ODF after the second refinement.
electronic reprint

(11) Omit all points of the refined
grids rðkþ1Þiji2 S2, i ¼ 1; . . . ;N, ji =
1; . . . ; Jðkþ1Þi , that do not satisfy therefinement criteria.
(12) Set k kþ 1 and continuewith step 5.
3. Practical example
The automated adaptive control of the
texture goniometer, in particular its
geometrical elements of successive
local refinement of the specimen
directions for which intensities are to
be measured, will be presented and
explained with the following case
study. We analyse a molybdenum
specimen with cubic crystal symmetry
Gcub with a Siemens–Bruker D5000
diffractometer with a Huber goni
ometer, restricting ourselves to the
four crystal forms fhk‘g ¼f200g; f110g; f211g; f321g.
Starting with the initial resolution
�ð1Þ = 20, we construct approximateequidistributions of specimen direc
tions rð1Þiji2 S2, i ¼ 1; . . . ; 4, ji ¼
1; . . . ; 54, with maximum azimuthangle � = 80. The maximum azimuthangle is a result of restrictions of the
experimental design. Using the ability
of the goniometer to measure diffrac
tion intensities for arbitrary arrange
ments of specimen directions, we
determine diffraction data ð�ð1Þiji ,hi; r
ð1ÞijiÞ, i ¼ 1; . . . ; 4, ji ¼ 1; . . . ; 54.
These data are plotted in the first row
of Fig. 3.
Following the flow chart of the
automated adaptive control algorithm, we fix an approximate
equidistribution gð1Þ1 ; . . . ; g
ð1Þ204 in SOð3Þ=Gcub with resolution
32 �ð1Þ = 30. As ansatz function ð1Þ, we choose the de la Vallée
Poussin kernel with halfwidth bð1Þ = 20. Now the PDFtoODF inversion algorithm is applied and a first estimated ODF
f̂f ð1Þ is obtained as a linear combination of the ansatz function ð1Þ shifted into the grid rotations gð1Þ1 ; . . . ; g
ð1Þ204. A plot of this
ODF is given in Fig. 5. Plots of computed pole figures can be
found in the top row of Fig. 4.
These computed pole figures are used in the refinement step
to define a grid of additional specimen directions rð2Þiji2 S2,
i ¼ 1; . . . ; 4, ji ¼ 1; . . . ;Nð2Þi , individually for each pole figure.For this purpose each initial grid is refined to have the reso
lution �ð2Þ ¼ 12 �ð1Þ = 10, but then only those specimen directions are retained for which the value of the computed PDF
exceeds the threshold value of 1.
Next, diffraction intensities ð�ð2Þiji ; hi; rð2ÞijiÞ, i ¼ 1; . . . ; 4,
ji ¼ 1; . . . ;Nð2Þi , with respect to the additional specimen
directions are measured. A plot of these together with
previously measured diffraction intensities can be found in the
second row of Fig. 3. Successive calculations of estimations of
the ODF, refinements of the grid of specimen directions, and
measurements of the corresponding diffraction intensities
result in progressively refined sets of diffraction data
ð�ðkÞiji ; hi; rðkÞijiÞ, i ¼ 1; . . . ; 4, ji ¼ 1; . . . ;NðkÞi , k ¼ 1; . . . ; 5,
plotted in Fig. 3, and progressively refined ODF estimates
f̂f ð1Þ; . . . ; f̂f ð5Þ. The estimated ODFs are plotted in Figs. 5–9, andthe computed pole figures are plotted in Fig. 4. In order to plot
ODFs, we use � sections as described by Helming et. al. (1988).More precisely, any individual section of the ODF f is a
spherical plot of the function ð; �Þ7!f ð; �; � � Þ with afixed value for �. Here ð; �; Þ denote the Euler anglerepresentation of a rotation according to the conventions used
by Helming et al. (1988).
In Table 1 the parameters of the individual steps are
summarized. The first column displays the angular resolution �
research papers
J. Appl. Cryst. (2007). 40, 570–579 Helmut Schaeben et al. � ODFcontrolled PDF measurements 577
Figure 8Estimated ODF after the third refinement.
electronic reprint

of the grid of specimen directions rðkÞiji
used in step
k ¼ 1; . . . ; 5, and the second column displays the resultingtotal number �NN of measured diffraction intensities withrespect to the locally refined grids. This total number of
measured intensities is compared with the total number �NNreg ofspecimen directions for a conventional, regular grid on the
hemisphere S2þ displayed in the third column. The cumulativetime spent to perform the measurements up to each step is
displayed in the fourth column. Since the measurement time
almost linearly increases with the number of measured
diffraction intensities, we conclude that we have time savings
of up to 75% or 150 h (step five). The time savings of about
40% in the third step of the successive refinement corresponds
almost exactly to the time savings observed previously
(Tarkowski et al., 2004) when comparing equalangle and
equalarea, i.e. approximately uniform grids.
The fifth column displays the
number MðkÞ of ansatz functions �½ ðgðkÞm Þ�1�, m ¼ 1; . . . ;MðkÞ, usedfor the representation of the ODF
estimate f̂f ðkÞ in step k. In column sixthe maximum order of the harmonic
series expansion, LðkÞ (‘bandwidth’) isspecified to which the ansatz functions
are restricted to allow for fast Fourier
techniques. The computational time
for the PDFtoODF inversion was
measured on a notebook with Intel
Core 2 Duo processor with 1.86 GHz
c.p.u. frequency and 2 Gbyte of
memory. Obviously, the computational
time is negligible compared with the
time savings during the measurement
process.
It should be noted that the c.p.u.
time increases by a factor of 23 ¼ 8from one refinement to the next,
except for the last refinement, as it
depends only on the spatial resolution
of the grid of SOð3Þ which is successively doubled, and not on the total
number of measured intensities �NN. Inthe last step, a lack of memory caused
additional computations and memory
swapping. With sufficiently large
memory the c.p.u. time could be
reduced from 31 h to approximately
4 h.
4. Conclusions
Using a novel method of PDFtoODF
inversion and an implementation
employing fast Fourier transform
algorithms, we have removed obsolete
restrictions such as seriously bounded
series expansion degree, seriously
research papers
578 Helmut Schaeben et al. � ODFcontrolled PDF measurements J. Appl. Cryst. (2007). 40, 570–579
Figure 9Estimated ODF after the fourth refinement.
Table 1Parameters for single refinement and recalculation steps.
Included are the resolution � of the grid of specimen directions of S2, thecumulative total number �NN of measured diffraction intensities with respect tothe locally refined grids, the total number �NNreg of diffraction intensities to bemeasured in a conventional experiment with a regular grid, the cumulativemeasurement time, the total number M of ansatz functions involved in thePDFtoODF inversion problem, the maximum order of harmonic seriesexpansion (bandwidth) L of the ansatz functions, and the computational timeto solve the PDFtoODF inversion problem with Core 2 Duo c.p.u. with186 GHz c.p.u. frequency and 2 Gbyte RAM.
Step � () �NN �NNregMeasurement
time (h) M LC.p.u.
time
1 20 216 288 0.60 21 23 3 s2 10 443 1152 1.23 204 52 28 s3 5 1621 4608 4.50 1493 108 209 s4 2.5 5511 18432 15.30 11767 215 1600 s5 1.25 19191 73728 53.30 94040 432 31 h
electronic reprint

bounded total number of components, regular spherical grid
of measurements on the pole sphere, weak to moderate
textures, and large c.p.u. times. Since it is now possible to
process intensity data of arbitrary location on the pole sphere
and successively compute numerical approximations of an
ODF, explaining the data while making measurements, we
suggest an automated adaptive control of a texture goni
ometer which either largely decreases the measuring time or
makes best use of the available measuring time. This tech
nique is especially well suited to the capture, representation
and analysis of extremely sharp textures, as in technical single
crystals.
The authors, in particular RH, gratefully acknowledge
financial support by Deutsche Forschungsgemeinschaft (grant
‘high resolution texture analysis’, PR 331/11, SCHA 465/15).
References
Bardsley, J. M. & Vogel, C. R. (2003). SIAM J. Sci. Comput. 25, 1326–1343.
Bukharova, T. I. & Savyolova, T. I. (1985a). Ind. Lab. 51, 56–60.Bukharova, T. I. & Savyolova, T. I. (1985b). J. Appl. Math. Math.Phys. 25, 617–622.
Bunge, H. J. (1965). Z. Metallkd. 56, 872–874.Eschner, T. (1993). Textures Microstruct. 21, 139–146.Eschner, T. (1994). Textures in Geological Materials, edited by H. J.
Bunge, S. Siegesmund, W. Skrotzki & K. Weber, pp. 15–28,Proceedings of a Workshop. Oberursel: DGM Informationsgesellschaft.
Grewen, J. & Wassermann, G. (1955). Acta Metall. 3, 354–360.
Helgason, S. (1984). Groups and Geometric Analysis. San Diego:Academic Press.
Helgason, S. (1999). The Radon Transform, 2nd ed. Boston:Birkhäuser.
Helming, K. & Eschner, T. (1990). Cryst. Res. Technol. 25, K203–K208.
Helming, K., Matthies, S. & Vinel, G. W. (1988). Proceedings of the 8thInternational Conference on Textures of Materials 1987, edited byJ. S. Kallend & G. Gottstein, pp. 55–60. Littleton: AmericanInstitute of Mining, Metallurgical, and Petroleum Engineers.
Hielscher, R. (2007). PhD Thesis, TU Freiberg, Germany.Hielscher, R., Bernstein, S., Schaeben, H., Boogaart, K. G. V. D.,
Beckmann, J. & Prestin, J. (2005). Mater. Sci. Forum, 495–497, 313–318.
Hielscher, R. & Schaeben, H. (2006). Proceedings IAMG 2006, Liège,September 3–8, 2006, CD S0612, 1p.
Lücke, K., Pospiech, J., Jura, J. & Hirsch, J. (1986). Z. Metallkd. 77,312–321.
Lücke, K., Pospiech, J., Virnich, K. H. & Jura, J. (1981). Acta Metall.29, 167–182.
Matthies, S. (1979). Phys. Status Solidi B, 92, K135–K138.Nikolayev, D. I., Savyolova, T. I. & Feldmann, K. (1992). TexturesMicrostruct. 19, 9–27.
Roe, R. J. (1965). J. Appl. Phys. 36, 2024–2031.Schaeben, H. (1996). J. Appl. Cryst. 29, 516–525.Schaeben, H. (1997). Phys. Status Solidi B, 200, 367–376.Schaeben, H. (1999). Textures Microstruct. 33, 365–373.Schaeben, H. (2000). J. Struct. Geol. 22, 1565–1568.Schaeben, H. & Boogaart, K. G. V. D. (2003). Tectonophysics, 370,
253–268.Tarkowski, L., Laskosz, L. & Bonarski, J. T. (2004). Mater. Sci. Forum,443–444, 137–140.
Virnich, K. H., Pospiech, J., Flemmer, A. & Lücke, K. (1978).Proceedings of ICOTOM 5, edited by G. Gottstein & K. Lücke, pp.129–138. Berlin: Springer Verlag.
research papers
J. Appl. Cryst. (2007). 40, 570–579 Helmut Schaeben et al. � ODFcontrolled PDF measurements 579electronic reprint